On October 23rd, 2014, we updated our
By continuing to use LinkedIn’s SlideShare service, you agree to the revised terms, so please take a few minutes to review them.
Chaudhari Y D / International Journal Of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.317-321 Investigation Of Tool Wear In Hard Turning Using Taguchi Method Chaudhari Y D 1 Mechanical Engineering Department, Sankalchand Patel College Of Engineering, Visnagar, Gujarat, 384 315.ABSTRACT Hard turning is a machining process investigate the tool life to assure the economicdefined of hardness higher than 45 HRC under justification for hard turning. As reported by Byrneappropriate cutting tools and cutting speed. The et al.  and Klocke et al. , the hard turning canobjective of this paper is to investigate the provide a relatively high accuracy for hardenedoptimum process parameters for a particular components but the problems occur with surfacework piece-tool material combination. . In this finish and tool wear.The design of experiment is astudy, three levels of each parameters viz. significant tool for Improvement of productionHardness (HRC), Speed(mm/min), Feed(mm/rev) process in engineering world. Firstly, in the 1920s, itand three different tool materials are evaluated was used by an English statistician Sir Ranoldfor process quality characteristics such as tool Fisher. Then, in Japan, new arrangements werewear. The three different tool materials used are made by Professor Genici Taguchi so that theHigh CBN, Low CBN, Mixed ceramic. AISI H 11 method can be used in the production sector.was taken as work piece material. The Taguchi method is a method of the experimentalexperiment is designed using Taguchi Method. design in which the variability in the product orThe results obtained from the experiments are process minimizes, choosing the optimum levels andtransformed into signal to noise (S/N) ratio and combinations of controllable factors against factorsused to optimize the value of tool wear. The which the variability forms uncontrolled factors.analysis of variance (ANOVA) is performed to The method is straightforward, easy to follow, andindentify the statistical significance of needs no guesswork to take the initial experimentalparameters. The final results of experimental steps. It relies on the assignment of factors ininvestigation are presented in this paper. The specific orthogonal arrays to determine these testconclusions arrived at are critically discussed at combinations. This approach facilitates thethe end. identification of the influence of individual factors establishing the relationship between factors andKeywords: Hard turning, Taguchi Technique, operational conditions, and finally establishingANOVA, Surface Finish, Flank Wear. performance at the optimum levels obtained. The Taguchi method not only helps in savingINTRODUCTION considerable time and cost, but also leads to a more Precision hard turning, an alternative to fully developed process. However, by applyingconventional grinding, is a cost-effective, high Taguchi method, only effective parameters andproductivity and flexible machining process for their interactions are determined, but no ultimateferrous metal components, which are often hardened values for optimum parameters are obtained.above 45 HRC [1,2]. The material removal rate Therefore, it is necessary that multiple level(MRR) in hard turning is much higher than grinding experiments are conducted in order to determineeven though smaller depth of cut and feed rates are optimum parameters .required . It has also been reported that the Taguchi recommends the use of the S/Nresulting machining time reduction is as high as ratio for the determination of the quality60% in hard turning . The turning of hardened characteristics implemented in engineering designcomponents are used in many applications such as problems. The S/N ratio characteristics can begears, shafts, bearings, cams, forgings, dies and divided into three stages: smaller the better, nominalmolds, which significantly reduce the manufacturing the best, and larger the better, signed–targetcosts, lead times and improve overall product type.Since the purpose of this study is to minimizequality [5–8]. surface roughness within the optimal levels of The hard turning is generally performed process parameters, the smaller the better qualitywithout a coolant using ceramics and cubic boron characteristic is selected. In addition to the S/Nnitride (CBN) cutting tools due to the required tool ratio, a statistical analysis of variance (ANOVA)material hardness. The cutting tools required for can be employed to indicate the impact of processhard turning are relatively expensive as compared to parameters on surface roughness. In this way, thegrinding operations and hence there is a need to 317 | P a g e
Chaudhari Y D / International Journal Of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.317-321optimal levels of process parameters can be achieving 45HRc.similarly another two bar tempera 600o and 560oc temperature for achieving 50 andTable: 2.2. L9 Orthogonal array 54HRc respectively. The experiment is designed using Taguchi method using three factors and eachExp. Tool Hardness Speed Feed factor is considered at three levels as shown in tableNo. material (HRC) (m/min) (mm/rev) 2.1. High1 45 180 0.12 Table: 2.1. Variable factors and their level CBN High Level Level2 50 230 0.15 Factor Column Level 3 CBN 1 2 High Tool High Low Mixed3 54 250 0.30 A CBN material CBN CBN ceramic Low Hardness4 45 230 0.30 B 45 50 54 CBN (HRC) Low Speed5 50 250 0.12 C 180 230 250 CBN (mm/min) Low Feed6 54 180 0.15 D 0.12 0.15 0.30 CBN (mm/rev) Mixed7 45 250 0.15 L9 orthogonal array is employed which is ceramic Mixed shown in table 2.2.three inserts we have selected for8 50 180 0.30 machining on different work piece material. ceramic Mixed KBN10B-TNGA160408S01225SE Low CBN9 54 230 0.12 content insert, KBN65B-TNGA 160408T01215SE ceramic High content CBN insert and mixed ceramic inserts.estimated. the experimental tool wear measure by using profile Many machining factors affect the quality projector and surface roughness measure on surfacecharacteristics of TURNING process. Taguchi roughness tester.method can provide efficient evaluation than thetraditional factorial design in experiment with fewertrials and low cost. Several researches have 2. TOOL WEAR RATIO:investigated the TURNING performance using Prediction of tool wear is complex becauseTaguchi method [12-17]. of the complexity of machining system . ToolT. Tamizharasan · T. Selvaraj · A. Noorul wear in cutting process is produced by the contactHaq.used Taguchi method to determine tool and relative sliding between the cutting tool and theflank wear,material removal rate and tool life by work piece and between the cutting tool and the chipusing different hardness of work piece and different under the extreme conditions of cutting area;grade of CBN tool. temperature at the cutting edge can exceed 530°CThis paper investigates the optimization of process and pressure is greater than 13.79 N/mm2. Anyparameters for work piece material AISI H11 at element changing contact conditions in cutting areadifferent hardness and different tool material to affects tool wear. In my study the tool flank wearobtain the performance with tool wear at the measured on profile projector (SCOPE II -355H) atselected machining parameters using Taguchi differene cutting time shown in Table 3.1.method for CNC turning. Table 3.1 Flank wear readings1. EXPERIMENTAL PROCEDURE Exp Flank wear (mm) The AISI H11 work piece material is . 1 2 3 3.45 minselected and the composition of work piece material No. min min Minis as follows: C-0.33-0.44, Mn-0.20-0.50, Si-0.8- 1 0.072 0.103 0.210 0.2451.20, Cr- 4.75-5.50, P<0.03, Ni<0.3, Mo-1.10-1.60, 2 0.083 0.154 0.214 0.289V-0.3-0.6, Cu<0.25, S <0.03%. we have taken three 3 0.165 0.224 0.244 0.296different bars of work piece material having equal 4 0.068 0.099 0.127 0.225length of 250 mm and 50 mm diameter. After equal 5 0.067 0.100 0.149 0.248length of three parts were sent to achieve different 6 0.150 0.250 0.278 0.312hardness by heat treatment process (Viz. 45, 50, 54 7 0.167 0.217 0.273 0.354HRC). Generally, the heat treatment process 8 0.108 0.214 0.270 0.344includes steps of operations like annealing, 9 0.186 0.227 0.268 0.321hardening, quenching and tempering. The material isheat treated 1030oc upto 30min and then oil quench The results are analyzed by the S/N ratio. These are60o to 80oc and then tempering 630oc for one hour 9 different combinations as shown in the table 3.1. 318 | P a g e
Chaudhari Y D / International Journal Of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.317-321Each experiment is performed four different times.In practice, the S/N ratio of particular ratio is to be 3.1 Response table and response diagram forhigh as per the Taguchi method. . Since, for tool Flank wear:wear, quality depends on smaller the better and thus The response table, which contains the sum of allvalue of S/N ratio can be calculated by Minitab 15. S/N ratio of each level and for each factor. TheThe S/N ratio for each of experiments in given in response table (table: 3.2) shows the sum of S/Ntable 3.2 as given below. ratio for each level and each factor.Table 3.2 S/N Ratio for Flank wear Table 3.3 Response table for Flank wearExp.no Avg flank S/N ratio Level A B C D1 16.0544 1 14.46 15.26 13.60 15.03 0.1575 2 15.63 14.76 14.81 12.912 0.1850 14.6566 3 12.20 12.28 13.88 14.343 0.2322 12.6809 Delta 3.43 2.97 1.21 2.124 17.7379 Rank 1 2 4 3 0.12975 0.1410 17.01566 0.2475 12.12857 0.2527 11.94628 0.2340 12.61579 0.2505 12.0238 Fig. 1 Main effect plot for S/N Ratio.The graph prepared from response table 3.3, which Analysis of variance for Flank wear shown inshows that highest sum of S/N ratio is given by A2- Table 3.5.B1-C2-D1 indicated by yellow mark.Therefore the following are the optimumparameters are shown in table-3.4.Table-3.4 Optimum conditionsTool material Hardness Speed FeedLow CBN 45 230 0.12 319 | P a g e
Chaudhari Y D / International Journal Of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.317-321 Table 3.5 Analysis of Variance for Flank wear. Factor S.S D.F M.S F %P A 1.2123 2 0.6061 1 2.47% B 21.179 2 10.589 17.470 43.30% C 7.722 2 3.861 6.370 15.78% D 18.792 2 9.3960 15.502 38.42% Error 0 - Total 48.9053 8 - 100 Pooled error 1.2123 4 0.6061 -4. CONCLUSION: 4. Tonshoff HK, Wobker HG, Brandt D. Taguchi method is generally used to Hard turning–Influence on the workpieceidentify the best optimum parameter and find the properties. Trans NAMRI/SMEfactor, which is most effecting on the process. So 1995;23:215–20.here we have tried to identify the main optimum 5. Zou JM, Anderson M, Stahl JE.parameter. Identification of cutting errors in precision Similarly, for tool wear optimum condition hard turning process. J Mater Process can be achieved with work piece of 45HRC Tech 2004;153–154:746–50. while using High CBN tool bit at speed of 6. Rech J, Moisan A. Surface Integrity in 230 mm/min and feed of 0.12 mm/rev. finish hard turning of case hardened steels. The most affecting parameter on tool wear is Int J Mach Tool Manuf 2003;43:543–50. hardness which has impact of about 43.30%. 7. Destefani J. Technology key to mold making success.Manuf Eng5. FUTURE SCOPE 2004;133(4):59 64. Hard turning process is a very important 8. Elbestawi MA, Chen L, Becze CE, EI- machining process. Still there is lots of work Wardany TI. High-speed milling of dies can be done like measurements of force and and molds in their hardened state. Ann pressure components by using tool force CIRP 1997;46(1):57–62. dynamometer, measurements of tool wear by 9. Byrne G, Dornfeld D, Denkena B. using machine vision technology, Advancing cutting technology. Ann CIRP measurement of wear by using 2003;52(2):483–507. SEM(scanning electron microscope) . 10. Klocke F, Brinskmeier E, Weinert K. Capability profile of hard cutting and By doing above investigation we can get the grinding processes.Ann CIRP detail idea about the proper speed, depth of 2005;54(2):557–80. cut and feed and we can apply it for machining of various hardened materials 11. Asli Secilmis, A. Murat Olmez, Murat with different level of machining. Dilmec, H. Selcuk Halkaci, Ozgur Inan, “Determination of optimal EDM machining parameters for machined pure Someone can make Higher order titanium-porcelain adhesion” Int J Adv Mathematical model for Flank wear and Manuf Technol (2009) 45:55–61. crater wear and surface Roughness. 12. S.Thamizhmanii, S. Saparudin, S.6. Acknowledgement Hasan.”Analyses of surface roughness byThe authors wish special thanks to Motif engg. Pvt turning process using Taguchi method”limited ahmedabad for given permission to conduct Journal of Achievements in Materials andexperimental work during research. Manufacturing Engineering 13. Hasan O ktem Tuncay ErzurumluREFERENCES: Mustafa Col “A study of the Taguchi 1. Konig W, Berktold A, Koch KF. Turning optimization method for surface roughness versus grinding–a comparison of surface in finish milling of mold surfaces” Int J integrity aspects and attainable accuracies. Adv Manuf Technol (2006) 28: 694–700. Ann CIRP 1993;42(1):39–43. 14. SThamizhmanii, K. Kamarudin, E. A. 2. Tonshoff HK, Arendt C, Ben Amor R. Rahim, A. Saparudin, Cutting of hardened steel. Ann CIRP S.Hasan”Optimizing Surface Roughness 2000;49(2):547–66. and Flank Wear on Hard Turning Process 3. Tonshoff HK, Wobker HG, Brandt D. Using Taguchi Parameter Design” Tool wear and surface integrity in hard Proceedings of the World Congress on turning. Prod Eng 1996;3(1):19–24. Engineering 2007 Vol II. 320 | P a g e
Chaudhari Y D / International Journal Of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 3, Issue 2, March -April 2013, pp.317-32115. Bala Murugan Gopalsamy, Biswanath Mondal and sukmal “Taguchi Method and ANOVA an approach for process parameters optimization of hard machining while machining hardened steel” Journal of scientific and industrial research (2009).16. Guey-Jiuh Tzou, Ding-Yeng Chen, Chun- Yao Hsu”Application of Taguchi method in the optimization of cutting parameters for turning operations”17. Hari Singh “Optimizing Tool Life of Carbide Inserts for Turned Parts using Taguchi’s Design of Experiments Approach” Proceedings of the International MultiConference of Engineers and Computer Scientists 2008 Vol II IMECS 2008.18. T. Tamizharasan · T. Selvaraj · A. Noorul Haq “Analysis of tool wear and surface finish in hard turning” Int J Adv Manuf Technol (2006) 28: 671–679. 321 | P a g e